Isolation and characterization of [5,6]-pyrrolidino-Sc3N@Ih-C80 diastereomers
Yutaka Maeda; Masato Kimura; Chihiro Ueda; Michio Yamada; Toru Kikuchi; Mitsuaki Suzuki; Wei-Wei Wang; Naomi Mizorogi; Nikolaos Karousis; Nikos Tagmatarchis; Tadashi Hasegawa; Marilyn M. Olmstead; Alan L. Balch; Shigeru Nagase; Takeshi Akasaka; Chem.Commun. 50 (2014) 12552–; doi:10.1039/C4cc04946B

data_7115761
_publ_section_title
;
 Isolation and characterization of [5,6]-pyrrolidino-Sc3N@Ih-C80
 diastereomers
;
_journal_name_full               Chem.Commun.
_journal_page_first              12552
_journal_paper_doi               10.1039/C4cc04946B
_journal_volume                  50
_journal_year                    2014
_chemical_formula_moiety         'C88 H15 N2 O2 Sc3'
_chemical_formula_sum            'C88 H15 N2 O2 Sc3'
_chemical_formula_weight         1266.90
_chemical_name_common            '[5,6]-pyrrolidino-Sc3N@C80(2a)'
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014
_cell_angle_alpha                90
_cell_angle_beta                 96.297(4)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.156(4)
_cell_length_b                   21.026(6)
_cell_length_c                   21.582(7)
_cell_measurement_reflns_used    7447
_cell_measurement_temperature    90(2)
_cell_measurement_theta_max      28.23
_cell_measurement_theta_min      4.15
_cell_volume                     5032(3)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      90(2)
_diffrn_detector_area_resol_mean 8.33
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.975
_diffrn_measurement_device_type  'Bruker Apex II'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_unetI/netI     0.1186
_diffrn_reflns_Laue_measured_fraction_full 0.985
_diffrn_reflns_Laue_measured_fraction_max 0.975
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            27590
_diffrn_reflns_point_group_measured_fraction_full 0.985
_diffrn_reflns_point_group_measured_fraction_max 0.975
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.958
_diffrn_reflns_theta_min         4.150
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    0.462
_exptl_absorpt_correction_T_max  0.7458
_exptl_absorpt_correction_T_min  0.5301
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2012)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.672
_exptl_crystal_description       block
_exptl_crystal_F_000             2544
_exptl_crystal_size_max          0.280
_exptl_crystal_size_mid          0.160
_exptl_crystal_size_min          0.120
_platon_squeeze_details
;
TITL ms0056    P 21/c       R = 0.24
CELL   11.1560   21.0260   21.5820     90.00     96.30     90.00
SPGR P21/c
C101 0.895 0.518 0.166 !       8.93 eA-3
C102 0.050 0.091 0.700 !       4.94 eA-3
C103 0.078 0.079 0.646 !       4.90 eA-3
C104 0.640 0.968 0.535 !       3.61 eA-3
C105 0.097 0.438 0.116 !       3.58 eA-3
C106 0.672 0.988 0.515 !       3.55 eA-3
C107 0.986 0.470 0.162 !       3.24 eA-3
C108 0.187 0.938 0.498 !       2.73 eA-3
C109 0.548 0.484 0.990 !       2.66 eA-3
C110 0.823 0.533 0.935 !       2.36 eA-3
C111 0.794 0.483 0.986 !       2.34 eA-3
Q112 0.985 0.173 0.489 !       1.41 eA-3
Q113 0.155 0.717 0.837 !       1.26 eA-3
Q114 0.204 0.388 0.636 !       1.00 eA-3
Q115 0.640 0.171 0.390 !       0.97 eA-3
Q116 0.863 0.658 0.081 !       0.96 eA-3
Q117 0.090 0.063 0.144 !       0.94 eA-3
Q118 0.316 0.783 0.292 !       0.93 eA-3
Q119 0.252 0.080 0.143 !       0.93 eA-3
Q120 0.827 0.175 0.767 !       0.92 eA-3
Q121 0.903 0.518 0.639 !       0.90 eA-3
Q122 0.157 0.753 0.382 !       0.90 eA-3
Q123 0.859 0.199 0.307 !       0.90 eA-3
Q124 0.672 0.283 0.717 !       0.90 eA-3
Q125 0.668 0.189 0.802 !       0.90 eA-3
Q126 0.290 0.318 0.018 !       0.89 eA-3
Q127 0.342 0.983 0.918 !       0.88 eA-3
Q128 0.229 0.677 0.162 !       0.88 eA-3
Q129 0.450 0.690 0.137 !       0.87 eA-3
Q130 0.530 0.139 0.682 !       0.87 eA-3
Q131 0.657 0.156 0.244 !       0.87 eA-3
Q132 0.657 0.344 0.755 !       0.87 eA-3
Q133 0.067 0.668 0.172 !       0.87 eA-3
Q134 0.122 0.672 0.371 !       0.85 eA-3
Q135 0.409 0.140 0.128 !       0.85 eA-3
Q136 0.827 0.684 0.369 !       0.85 eA-3
Q137 0.576 0.907 0.973 !       0.84 eA-3
Q138 0.658 0.998 0.267 !       0.83 eA-3
Q139 0.561 0.345 0.201 !       0.83 eA-3
Q140 0.279 0.625 0.444 !       0.83 eA-3
Q141 0.267 0.457 0.333 !       0.82 eA-3
Q142 0.532 0.419 0.511 !       0.82 eA-3
C143 0.126 0.498 0.007 !       0.82 eA-3
Q144 0.982 0.765 0.346 !       0.82 eA-3
Q145 0.266 0.846 0.245 !       0.81 eA-3
Q146 0.874 0.155 0.801 !       0.81 eA-3
Q147 0.237 0.596 0.250 !       0.80 eA-3
Q148 0.451 0.316 0.731 !       0.80 eA-3
Q149 0.440 0.861 0.031 !       0.80 eA-3
Q150 0.359 0.168 0.878 !       0.79 eA-3
Q151 0.701 0.255 0.700 !       0.79 eA-3
Q152 0.359 0.379 0.200 !       0.78 eA-3
Q153 0.532 0.551 0.386 !       0.78 eA-3
Q154 0.880 0.343 0.494 !       0.77 eA-3
Q155 0.548 0.752 0.653 !       0.77 eA-3
Q156 0.937 0.733 0.435 !       0.77 eA-3
Q157 0.439 0.280 0.170 !       0.77 eA-3
Q158 0.295 0.455 0.670 !       0.76 eA-3
Q159 0.562 0.811 0.184 !       0.76 eA-3
Q160 0.449 0.690 0.888 !       0.76 eA-3
Q161 0.497 0.843 0.802 !       0.76 eA-3
Q162 0.347 0.781 0.892 !       0.75 eA-3
Q163 0.124 0.265 0.058 !       0.75 eA-3
Q164 0.715 0.843 0.965 !       0.75 eA-3
Q165 0.733 0.862 0.838 !       0.74 eA-3
Q166 0.281 0.172 0.793 !       0.74 eA-3
Q167 0.323 0.326 0.069 !       0.73 eA-3
Q168 0.771 0.374 0.480 !       0.73 eA-3
Q169 0.292 0.248 0.252 !       0.73 eA-3
Q170 0.904 0.784 0.257 !       0.73 eA-3
Q171 0.427 0.690 0.817 !       0.73 eA-3
Q172 0.315 0.752 0.479 !       0.73 eA-3
Q173 0.392 0.562 0.842 !       0.73 eA-3
Q174 0.079 0.173 0.538 !       0.73 eA-3
Q175 0.501 0.674 0.337 !       0.72 eA-3
Q176 0.670 0.578 0.622 !       0.72 eA-3
Q177 0.592 0.861 0.645 !       0.72 eA-3
Q178 0.675 0.251 0.523 !       0.71 eA-3
Q179 0.218 0.280 0.161 !       0.71 eA-3
Q180 0.454 0.968 0.294 !       0.71 eA-3
Q181 0.250 0.672 0.915 !       0.71 eA-3
Q182 0.465 0.140 0.104 !       0.71 eA-3
Q183 0.280 0.238 0.862 !       0.71 eA-3
Q184 0.311 0.889 0.342 !       0.71 eA-3
Q185 0.157 0.707 0.424 !       0.70 eA-3
Q186 0.179 0.641 0.019 !       0.70 eA-3
Q187 0.282 0.878 0.293 !       0.69 eA-3
Q188 0.110 0.610 0.336 !       0.69 eA-3
Q189 0.626 0.811 0.862 !       0.69 eA-3
Q190 0.694 0.700 0.944 !       0.69 eA-3
Q191 0.358 0.457 0.381 !       0.69 eA-3
Q192 0.826 0.296 0.116 !       0.69 eA-3
Q193 0.686 0.972 0.691 !       0.69 eA-3
Q194 0.248 0.673 0.016 !       0.69 eA-3
Q195 0.267 0.388 0.532 !       0.68 eA-3
Q196 0.906 0.609 0.600 !       0.68 eA-3
Q197 0.453 0.982 0.340 !       0.68 eA-3
Q198 0.489 0.124 0.963 !       0.68 eA-3
Q199 0.311 0.171 0.823 !       0.68 eA-3
Q200 0.423 0.217 0.260 !       0.68 eA-3
Q201 0.217 0.486 0.727 !       0.68 eA-3
Q202 0.671 0.376 0.338 !       0.67 eA-3
Q203 0.907 0.702 0.693 !       0.67 eA-3
Q204 0.221 0.559 0.405 !       0.67 eA-3
Q205 0.483 0.704 0.907 !       0.67 eA-3
Q206 0.408 0.830 0.360 !       0.67 eA-3
Q207 0.832 0.860 0.960 !       0.67 eA-3
Q208 0.890 0.125 0.832 !       0.67 eA-3
Q209 0.327 0.812 0.474 !       0.67 eA-3
Q210 0.518 0.782 0.491 !       0.66 eA-3
Q211 0.944 0.266 0.811 !       0.66 eA-3
Q212 0.731 0.332 0.926 !       0.66 eA-3
C213 0.068 0.088 0.320 !       0.66 eA-3
Q214 0.792 0.238 0.324 !       0.66 eA-3
Q215 0.065 0.704 0.091 !       0.66 eA-3
Q216 0.125 0.845 0.757 !       0.65 eA-3
Q217 0.484 0.700 0.297 !       0.65 eA-3
Q218 0.669 0.159 0.980 !       0.65 eA-3
Q219 0.064 0.159 0.165 !       0.65 eA-3
Q220 0.550 0.530 0.214 !       0.65 eA-3
Q221 0.391 0.768 0.878 !       0.65 eA-3
Q222 0.263 0.764 0.402 !       0.65 eA-3
Q223 0.738 1.002 0.710 !       0.65 eA-3
Q224 0.363 0.110 0.659 !       0.65 eA-3
Q225 0.330 0.876 0.707 !       0.65 eA-3
Q226 0.431 0.019 0.602 !       0.65 eA-3
Q227 0.105 0.935 0.044 !       0.65 eA-3
Q228 0.125 0.172 0.838 !       0.65 eA-3
Q229 0.701 0.880 0.699 !       0.65 eA-3
Q230 0.297 0.405 0.657 !       0.64 eA-3
Q231 0.936 0.377 0.001 !       0.64 eA-3
Q232 0.346 0.295 0.699 !       0.64 eA-3
Q233 0.145 0.187 0.307 !       0.64 eA-3
Q234 0.329 0.308 0.331 !       0.64 eA-3
Q235 0.625 1.003 0.796 !       0.64 eA-3
Q236 0.475 0.186 0.438 !       0.64 eA-3
Q237 0.317 0.495 0.649 !       0.64 eA-3
Q238 0.126 0.767 0.293 !       0.64 eA-3
Q239 0.123 0.513 0.391 !       0.64 eA-3
C240 0.957 0.482 0.922 !       0.64 eA-3
Q241 0.143 0.287 0.686 !       0.63 eA-3
Q242 0.238 0.673 0.557 !       0.63 eA-3
Q243 0.965 0.360 0.018 !       0.63 eA-3
Q244 0.697 0.734 0.768 !       0.63 eA-3
Q245 0.176 0.844 0.705 !       0.63 eA-3
C246 0.264 0.482 0.044 !       0.63 eA-3
Q247 0.028 0.487 0.494 !       0.63 eA-3
Q248 0.689 0.156 0.571 !       0.63 eA-3
Q249 0.300 0.799 0.433 !       0.62 eA-3
Q250 0.577 0.218 0.464 !       0.62 eA-3
Q251 0.019 0.280 0.207 !       0.62 eA-3
Q252 0.120 0.623 0.156 !       0.62 eA-3
Q253 0.315 0.143 0.137 !       0.62 eA-3
Q254 0.403 0.360 0.798 !       0.62 eA-3
Q255 0.374 0.299 0.356 !       0.62 eA-3
Q256 0.486 0.624 0.498 !       0.62 eA-3
Q257 0.892 0.750 0.266 !       0.62 eA-3
Q258 0.889 0.345 0.673 !       0.61 eA-3
Q259 0.342 0.857 0.890 !       0.61 eA-3
Q260 0.986 0.782 0.373 !       0.61 eA-3
Q261 0.550 0.950 0.730 !       0.61 eA-3
Q262 0.299 0.841 0.595 !       0.61 eA-3
Q263 0.545 0.670 0.738 !       0.61 eA-3
Q264 0.578 0.580 0.203 !       0.61 eA-3
Q265 0.985 0.377 0.379 !       0.61 eA-3
Q266 0.483 0.315 0.915 !       0.61 eA-3
Q267 0.629 0.824 0.292 !       0.61 eA-3
Q268 0.020 0.671 0.592 !       0.61 eA-3
Q269 0.638 0.532 0.815 !       0.61 eA-3
Q270 0.317 0.349 0.842 !       0.61 eA-3
Q271 0.752 0.734 0.186 !       0.60 eA-3
Q272 0.013 0.124 0.570 !       0.60 eA-3
Q273 0.954 0.672 0.987 !       0.60 eA-3
Q274 0.734 0.030 0.211 !       0.60 eA-3
Q275 0.597 0.736 0.387 !       0.60 eA-3
Q276 0.718 0.607 0.053 !       0.60 eA-3
Q277 0.330 0.185 0.018 !       0.60 eA-3
Q278 0.092 0.969 0.847 !       0.60 eA-3
Q279 0.601 0.236 0.754 !       0.60 eA-3
Q280 0.903 0.142 0.548 !       0.60 eA-3
Q281 0.598 0.767 0.879 !       0.60 eA-3
Q282 0.512 0.596 0.117 !       0.60 eA-3
Q283 0.063 0.924 0.492 !       0.60 eA-3
Q284 0.954 0.372 0.685 !       0.59 eA-3
Q285 0.677 0.693 0.085 !       0.59 eA-3
Q286 0.199 0.188 0.338 !       0.59 eA-3
Q287 0.670 0.559 0.834 !       0.59 eA-3
C288 0.889 0.031 0.515 !       0.59 eA-3
Q289 0.201 0.782 0.296 !       0.59 eA-3
Q290 0.516 0.061 0.287 !       0.59 eA-3
Q291 0.280 0.686 0.254 !       0.58 eA-3
Q292 0.858 0.500 0.377 !       0.58 eA-3
Q293 0.579 0.125 0.897 !       0.58 eA-3
Q294 0.095 0.371 0.524 !       0.58 eA-3
Q295 0.500 0.340 0.087 !       0.58 eA-3
C296 0.837 0.435 0.948 !       0.58 eA-3
Q297 0.465 0.828 0.661 !       0.58 eA-3
Q298 0.019 0.939 0.103 !       0.58 eA-3
Q299 0.266 0.685 0.576 !       0.58 eA-3
Q300 0.791 0.656 0.051 !       0.58 eA-3
Q301 0.872 0.455 0.323 !       0.58 eA-3
Q302 0.723 0.157 0.028 !       0.58 eA-3
Q303 0.491 0.683 0.931 !       0.58 eA-3
Q304 0.629 0.465 0.392 !       0.58 eA-3
Q305 0.816 0.780 0.377 !       0.58 eA-3
Q306 0.248 0.266 0.027 !       0.58 eA-3
Q307 0.386 0.737 0.916 !       0.58 eA-3
Q308 0.441 0.312 0.846 !       0.58 eA-3
Q309 0.973 0.156 0.596 !       0.58 eA-3
Q310 0.221 0.761 0.411 !       0.57 eA-3
Q311 0.120 0.800 0.270 !       0.57 eA-3
Q312 0.359 0.530 0.334 !       0.57 eA-3
Q313 0.169 0.738 0.146 !       0.57 eA-3
Q314 0.281 0.516 0.757 !       0.57 eA-3
Q315 0.579 0.486 0.244 !       0.57 eA-3
Q316 0.511 0.865 0.575 !       0.57 eA-3
Q317 0.063 0.314 0.282 !       0.57 eA-3
Q318 0.637 0.017 0.610 !       0.57 eA-3
Q319 0.917 0.190 0.554 !       0.57 eA-3
Q320 1.005 0.300 0.851 !       0.57 eA-3
Q321 0.267 0.200 0.142 !       0.57 eA-3
Q322 0.140 0.719 0.654 !       0.57 eA-3
Q323 0.096 0.891 0.126 !       0.57 eA-3
Q324 0.395 0.382 0.503 !       0.57 eA-3
Q325 0.604 0.921 0.315 !       0.57 eA-3
Q326 0.800 0.733 0.915 !       0.57 eA-3
Q327 0.890 0.139 0.397 !       0.56 eA-3
Q328 0.268 0.965 0.723 !       0.56 eA-3
Q329 0.876 0.236 0.400 !       0.56 eA-3
Q330 0.561 0.841 0.374 !       0.56 eA-3
Q331 0.613 0.287 0.077 !       0.56 eA-3
Q332 0.354 0.626 0.885 !       0.56 eA-3
Q333 0.532 0.213 0.696 !       0.56 eA-3
Q334 0.469 0.531 0.159 !       0.56 eA-3
Q335 0.561 0.833 0.100 !       0.56 eA-3
Q336 0.673 0.816 0.240 !       0.56 eA-3
Q337 0.121 0.784 0.582 !       0.56 eA-3
Q338 0.699 0.813 0.394 !       0.56 eA-3
Q339 0.918 0.801 0.111 !       0.56 eA-3
Q340 0.547 0.434 0.622 !       0.55 eA-3
Q341 0.301 0.904 0.030 !       0.55 eA-3
Q342 0.018 0.564 0.601 !       0.55 eA-3
Q343 0.217 0.936 0.127 !       0.55 eA-3
Q344 0.700 0.950 0.734 !       0.55 eA-3
C345 0.246 0.484 0.899 !       0.55 eA-3
Q346 0.608 0.110 0.462 !       0.55 eA-3
Q347 0.676 0.388 0.606 !       0.55 eA-3
Q348 0.734 0.782 0.207 !       0.55 eA-3
Q349 0.781 0.052 0.068 !       0.55 eA-3
Q350 0.781 0.501 0.567 !       0.55 eA-3
Q351 0.407 0.624 0.655 !       0.55 eA-3
Q352 0.718 0.015 0.325 !       0.55 eA-3
Q353 0.641 0.452 0.850 !       0.55 eA-3
Q354 0.858 0.778 0.928 !       0.55 eA-3
Q355 0.205 0.874 0.888 !       0.55 eA-3
Q356 0.593 0.203 0.929 !       0.55 eA-3
Q357 0.344 0.547 0.202 !       0.54 eA-3
Q358 0.736 0.701 0.129 !       0.54 eA-3
Q359 0.333 0.704 0.012 !       0.54 eA-3
Q360 0.155 0.813 0.262 !       0.54 eA-3
Q361 0.078 0.843 0.783 !       0.54 eA-3
Q362 0.278 0.409 0.593 !       0.54 eA-3
Q363 0.263 0.169 0.295 !       0.54 eA-3
Q364 0.128 0.173 0.974 !       0.54 eA-3
Q365 0.674 0.626 0.024 !       0.54 eA-3
Q366 0.387 0.749 0.777 !       0.54 eA-3
Q367 0.157 0.185 0.899 !       0.54 eA-3
Q368 0.171 0.877 0.485 !       0.54 eA-3
Q369 0.963 0.093 0.903 !       0.53 eA-3
Q370 0.626 0.642 0.022 !       0.53 eA-3
Q371 0.046 0.562 0.747 !       0.53 eA-3
Q372 0.626 0.145 0.680 !       0.53 eA-3
Q373 0.846 0.172 0.164 !       0.53 eA-3
Q374 0.050 0.173 0.064 !       0.53 eA-3
Q375 0.387 0.487 0.463 !       0.53 eA-3
Q376 0.489 0.889 0.245 !       0.53 eA-3
Q377 0.265 0.379 0.889 !       0.53 eA-3
Q378 0.668 0.642 0.115 !       0.53 eA-3
Q379 0.548 0.750 0.209 !       0.53 eA-3
Q380 0.689 0.139 0.310 !       0.53 eA-3
Q381 0.515 0.405 0.822 !       0.53 eA-3
Q382 0.235 0.298 0.594 !       0.53 eA-3
Q383 0.954 0.471 0.463 !       0.53 eA-3
Q384 0.173 0.187 0.736 !       0.53 eA-3
Q385 0.452 0.627 0.630 !       0.53 eA-3
Q386 0.468 0.706 0.862 !       0.52 eA-3
Q387 0.887 0.366 0.260 !       0.52 eA-3
Q388 0.536 0.500 0.872 !       0.52 eA-3
Q389 0.528 0.323 0.247 !       0.52 eA-3
Q390 0.624 0.874 0.375 !       0.52 eA-3
Q391 0.559 0.548 0.858 !       0.52 eA-3
Q392 0.094 0.358 0.567 !       0.52 eA-3
Q393 0.673 0.344 0.568 !       0.52 eA-3
Q394 0.577 0.841 0.739 !       0.52 eA-3
Q395 0.530 0.530 0.249 !       0.52 eA-3
Q396 0.312 0.048 0.377 !       0.52 eA-3
Q397 0.314 0.721 0.034 !       0.52 eA-3
Q398 0.046 0.878 0.810 !       0.52 eA-3
Q399 0.720 0.484 0.790 !       0.51 eA-3
Q400 0.612 0.107 0.142 !       0.51 eA-3
Q401 0.188 0.390 0.449 !       0.51 eA-3
Q402 0.849 0.611 0.450 !       0.51 eA-3
Q403 0.160 0.091 0.721 !       0.51 eA-3
Q404 0.978 0.078 0.871 !       0.51 eA-3
Q405 0.157 0.874 0.696 !       0.51 eA-3
Q406 0.844 0.434 0.835 !       0.51 eA-3
Q407 0.782 0.325 0.760 !       0.51 eA-3
Q408 0.191 0.235 0.806 !       0.51 eA-3
Q409 0.496 0.324 0.544 !       0.51 eA-3
Q410 0.891 0.268 0.698 !       0.51 eA-3
Q411 0.983 0.813 0.697 !       0.51 eA-3
Q412 0.919 0.409 0.284 !       0.51 eA-3
Q413 0.169 0.860 0.790 !       0.51 eA-3
Q414 0.361 0.627 0.981 !       0.50 eA-3
Q415 0.987 0.111 0.543 !       0.50 eA-3
Q416 0.858 0.018 0.212 !       0.50 eA-3
Q417 0.015 0.783 0.719 !       0.50 eA-3
Q418 0.741 0.636 0.544 !       0.50 eA-3
Q419 0.528 0.607 0.159 !       0.50 eA-3
Q420 0.420 0.373 0.714 !       0.50 eA-3
Q421 0.720 0.329 0.642 !       0.50 eA-3
Q422 0.232 0.285 0.730 !       0.50 eA-3
Q423 0.594 0.362 0.596 !       0.50 eA-3
;
_refine_diff_density_max         0.841
_refine_diff_density_min         -0.582
_refine_diff_density_rms         0.132
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.032
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1549
_refine_ls_number_reflns         27590
_refine_ls_number_restraints     1803
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.1587
_refine_ls_R_factor_gt           0.1246
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1567P)^2^+23.9482P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3414
_refine_ls_wR_factor_ref         0.3595
_reflns_Friedel_coverage         0.000
_reflns_number_gt                18535
_reflns_number_total             27590
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c4cc04946b2.cif
_cod_data_source_block           ms0056
_cod_database_code               7115761
_shelx_estimated_absorpt_t_min   0.882
_shelx_estimated_absorpt_t_max   0.947
_shelxl_version_number           2014-3
_shelx_res_checksum              69137